Upload
lamkhuong
View
292
Download
16
Embed Size (px)
1
PowerPoint Prepared By Ir Sam YipDate: 29 th April 2014
Optimizing Concrete Mix Design
Optimizing Concrete Mix Design
Content :
� Introduction
� Project Requirements in Concrete Design
� Concrete Mix Design
� Methodologies for Concrete Mix Design
� Difficulties and Constraints
� Quality Management System
2
Introduction
� Construction Industry is blooming in Hong Kong recently. Numerous projects are in progress include mega infrastructure project, MTRC Railway projects, Hong Kong Housing Authority projects, Government projects, high rise building etc.
� There is an increase in concrete demand.� More stringent in concrete mix design criteria and
requirements.� Require higher quality of concrete mixes.
3
Local Projects
� Hong Kong – Zhuhai – Macao Bridge Project
4
Local Projects
� Hong Kong – Zhuhai – Macao Bridge Project
5
Local Projects
� Stonecutters Bridge Project
6
Local Projects
� Wan Chai Reclamation Project
7
Local Projects
� MTRC XRL Project
8
Local Projects
� Tunneling Works for XRL Project
9
Local Projects
� Highway Project
10
Local Projects
� International Commercial Centre at West Kowloon
11
Local Projects
� Foundation Project
12
Project Requirements in Concrete Design
� In Hong Kong, there are numerous specifications for concrete, major specifications include • General Specifications for CEW• Building (Construction) Regulations• Hong Kong Housing Authority• Architectural Services Dept of HKSAR• MTRC• Hong Kong Electric & China Light Power• Ove Arup, AECOM, BV…• Various projects’ particular specifications……
13
Project Requirements in Concrete Design
� Different specifications have different concrete design requirements.
� There are inconsistent in the concrete requirements among different specifications. Examples include:• Max cementitious content for liquid retaining structure
• A Particular WSD project - 430kg/m3• G.S. - 450kg/m3• ASD - 440kg/m3
• Min cementitious content for Grade 20 Concrete (plain concrete)• B.D. - 290kg/m3• G.S. - 270kg/m3• ASD - 275kg/m3 14
Project Requirements in Concrete Design
� Recent projects aim for high performance concrete mix design to facilitate the concreting works to suit specific applications.
� Requirements include:• High compressive strength
For skyscraper and high rise building to maximize the useable floor area and slim structure
• DurabilityFor structure with long design life e.g. 120 years and lower the maintenance cost
15
Project Requirements in Concrete Design
• High workability concrete & retention propertiesTo facilitate the concreting works and for environmental protection purpose
• Early strength concreteTo shorten the working cycle and demoulding time
• Low heat of hydrationFor massive structure and prevent thermal effect
16
Project Requirements in Concrete Design
• Shrinkage reductionTo minimize shrinkage cracks in water retaining structure
• Anti-corrosion behaviourTo protect the embedded rebar against corrosion
• Other project special requirements…..
17
Project Requirements in Concrete Design
� Examples� Hong Kong – Zhuhai – Macao Bridge Project
• Limitation in max cementitious content of 450kg/m3
• Limitation in max water cement ratio of 0.38• Compliance in chloride diffusion test• Long workability retention time for marine
transportation• High PFA content (up to 40%) for durability
purpose
18
Project Requirements in Concrete Design
� Examples� HATS Project requirements
• Limitation in max cementitious content of 450kg/m3
• Limitation in max water cement ratio of 0.38• RCPT ≤ 1000 coulombs• Sorptivity ≤ 0.07 (mm/min1/2)• Long workability retention time for concrete
transit• Early strength for working cycle including
demoulding19
Project Requirements in Concrete Design
� Examples� Highway Project requirements
• High compressive strength (50MPa)• High early strength to reopen the road or
minimize the vibration effect (to achieve 12MPa within 4 hours)
20
Concrete Mix Design
� Concrete mix design is the process to select suitable constituent materials and determine required and specified characteristics of a concrete mixture.• Prescriptive approach • Performance approach
� Mix design requirements are based on intended use, exposure conditions etc.
21
Typical Concrete Mix Design Process
� Review of specification requirements for all constraints, e.g. materials, production, and construction methodologies
� Assessing availability of materials� Selection of materials to ensure the conformity with
standard and specifications� Obtaining data and/or testing of materials� Identifying influencing of mix design on concrete
production and construction materials� Obtaining approval for mix design
22
Basic Factors for Concrete Mix Design
� Grade and strength� Water cement ratio� Limitation in max / min cementitious content� Workability� Max aggregate size� Aggregate cement ratio� Durability considerations (exposure conditions)� Plastic density� Applications and construction methods including
the spacing of rebar� Etc.. 23
Methods for Concrete Mix Design
� There are many concrete mix design methods and commonly adopted methods include:
• Building Research Establishment of UK (BRE)• America Concrete Institute (ACI)• Volumetric Method
24
BRE Method
� Formerly developed by British Department of Environment (DOE)
� Applied only for normal weight concrete
� High performance concrete is not covered
� Principle:
- Use historical and available data
- Adopt charts and tables
Example:
Specified Requirement� For “OPC” Concrete:• Characteristic compressive str. (fc) = 45MPa at 28-day with
a 5% defective rate (k = 1.64)• Design Slump = 100mm• OPC Class = 52.5N• Max. aggregate size = 20mm• Type of fine aggregates = Crushed rock fines • Relative density of aggregate = 2.7 (SSD condition)• Past cube compression test result or production data is not available
�For “OPC + PFA” concrete:• Same as above with PFA of proportion (p) = 30%
BRE Method
BRE Method
fc=45
BRE Method
Mix with OPC
Mix withOPC + PFA (30%)
Step 1:Target mean strength f m
(Fig. 3)Margin M = k x s
= 1.64 x 8= 13 MPa
Target mean strength fm = fc + M
= 45 + 13= 58 MPa
(Fig. 3)Margin M = k x s
= 1.64 x 8= 13 MPa
Target mean strength fm = fc + M
= 45 + 13= 58 MPa
BRE Method(OPC & OPC+PFA Concrete)
55fm=58
0.48
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Step 2:Selection of target free-water/cement ratio
(Table 2 ; Fig. 4)Target free-water/cement ratio = 0.48
(Table 10 ; Fig. 4)W/(C+eF)where e is cementing efficiency factor = 0.30F = PFA contentTarget free W/(C+0.30F) = 0.48
BRE Method
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Step 3:Selection of free water content (W)
(Table 3)Free water content W = 225 kg/m 3
(Table 9)Free water content W = 225 - 20
= 205 kg/m 3
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Step 4:Determination of cement content (C)
PFA content (F) W/(C+F) ratio
Cement content C = 225/0.48
= 469 kg/m 3
Cement content (C)0.48 = 205 / (C+0.3F)Since F = C /0.7 x 0.3C = 378 kg/m 3
PFA content (F)F = C/ 0.7 x 0.3
= 162 kg/m 3
Thus, W/(C+F) = 205/(378+162) = 0.38
BRE Method
225
2385
205
2405
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Step 5:Determination of total aggregate content (SSD condition)
(Fig. 5)Wet density of concrete D = 2385 kg/m3
Total aggregate content (SSD) = D - C - W= 2385 - 469 – 225= 1691 kg/m3
(Fig. 5)Wet density of concrete D = 2405 kg/m3
Total aggregate content (SSD)= D - C - F - W= 2405 - 378 - 162 - 205= 1660 kg/m3
BRE Method
0.48
4735
0.38
44
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Step 6:Selection of fine and coarse aggregate contents
(Fig. 6)Proportion of fine aggregate = 47%
Fine aggregate content = 1691 x 0.47 = 795 kg/m3
Coarse aggregate content = 1691 - 795 = 896 kg/m3
20mm : 10mm ~ 2 : 120mm = 896 x 2/3
= 597 kg/m3
10mm = 896 x 1/3= 299 kg/m3
(Fig. 6)Proportion of fine aggregate = 44%
Fine aggregate content = 1660 x 0.44 = 730 kg/m3
Coarse aggregate content = 1660 - 730 = 930 kg/m3
20mm : 10mm ~ 2 : 120mm = 930 x 2/3
= 620 kg/m3
10mm = 930 x 1/3= 310 kg/m3
BRE Method
Mix withOPC
Mix withOPC + PFA (30%)
Preliminary Mix Design Proportion
OPC = 469 kg/m3
20mm = 597 kg/m3
10mm = 299 kg/m3
CRF = 795 kg/m3
Water = 225 kg/m3
Wet density = 2385 kg/m3
W/C = 0.48
OPC = 378 kg/m3
PFA = 162 kg/m3
20mm = 620 kg/m3
10mm = 310 kg/m3
CRF = 730 kg/m3
Water = 205 kg/m3
Wet density = 2405 kg/m3
W/(C+F) = 0.38
ACI Mix Design
� The most common method adopted in North America which is established by American Concrete Institute.
39
ACI Method
� Example� To design a concrete mix for an exterior column located
above ground where substantial freezing and thawing may occur.• Grade : 35MPa (~5000PSi)• Slump ~ 50mm (1 – 2 inch)• Max size aggregate: 20mm (~0.75 inch)• Cement: Type I, SG: 3.15• Coarse aggregate:
Bulk density (SSD) = 2.7; Absorption capacity = 1%, Oven dried unit weight = 100 lb/ft3; Surface moisture = 0
• Fine aggregate: Bulk density (SSD) = 2.65; Absorption capacity = 1.3%, Fineness modulus = 2.7, Surface moisture = 3%
40
ACI Mix Design
� Mix Design Procedure� Step 1 - Required material information
• Including sieve analysis for both coarse and fine aggregate, specific gravity etc.
� Step 2 – Choice of slump• Normally it is specified by the project. If not, it
can be chosen from Table to suit the application.
41
ACI Mix Design
� Recommended slumps for various types of construction
42
ACI Mix Design
� Step 3 - Maximum aggregate size• Maximum size should not be larger than:
• 1/5 the minimum dimension of structural members• 1/3 the thickness of a slab• 3/4 the clearance between reinforcement and
formwork
43
ACI Mix Design
� Step 4 - Estimating of mixing water and air content• An estimation of the amount of water required for
air entrained and non-air entrained concrete can be obtained from Table.
• Concrete is routinely air entrained in North America.
44
ACI Mix Design
45
ACI Mix Design
� Step 5 – Water / Cement Ratio• This component is governed by strength and
durability requirements.• Strength – Related to water cement ratio and
referred to 28 days compressive strength.• Durability – If there are severe exposure
conditions, such as freezing and thawing, exposure to seawater, or sulfates, the w/c ratio requirements may have to be adjusted.
46
ACI Mix Design
47
ACI Mix Design
� Step 6 - Calculation of cement content• Once the water content and the w/c ratio is
determined, the amount of cement per unit volume of the concrete is found by dividing the estimated water content by the w/c ratio.
• Weight of cement = Weight of water / (w/c)• Weight of cement = 280/0.4 = 700 (lb/yd3)
= 415 (kg/m3)Note: A minimum cement content is required to ensure good finishability, workability and strength.
48
ACI Mix Design
� Step 7 - Estimation of coarse aggregate content • The percent of coarse aggregate to concrete for
a given maximum size and fineness modulus is given in Table.
• The value from the table multiplied by oven dried weight of coarse aggregate required per cubic foot of concrete.
• Volume of coarse aggregate = 0.63 x 27 (ft3/yd3) = 17.01 (ft3/yd3)
• The oven dried weight of coarse aggregate= 17.01 (ft3/yd3) x 100 lb/ft3= 1,701 lb/yd3 (1,009 kg/m3) 49
ACI Mix Design
50
ACI Mix Design
� Step 8 - Estimation of fine aggregate content • There are two standard methods to establish the
fine aggregate content, the mass method and the volume method.
• Volume method – This method is the preferred method, as it is a somewhat more exact procedure.
• The volume of fine aggregate is found by subtracting the volume of cement, water, air and coarse aggregate from the total concrete volume.
51
ACI Mix Design
� Step 8 - Estimation of fine aggregate content • Water: 280 lb/ 62.4 lb/ft3 = 4.49 ft3
= 0.1271 m3
• Cement: 700 lb/(3.15 x 62.4 lb/ft3) = 3.56 ft3
= 0.1008 m3
• Coarse Agg: 1701 lb/(2.7 x 62.4 lb/ft3) = 10.10 ft3
= 0.2860 m3
• Air: 6% x 27ft3/yd3 = 1.62 ft3= 0.0459 m3
Total = 19.77 ft3= 0.5598 m3
52
ACI Mix Design
� Step 8 - Estimation of fine aggregate content • Fine aggregate occupied a volume of:
= 27 ft3 – 19.77 ft3 = 7.23 ft3 (0.2047m3)= 0.1271 m3
• Oven dried weight of fine aggregate:7.23 ft3 x 2.65 (SG) x 62.4 lb/ft3 (Unit weight of water)= 1,196 lb (544kg)
53
ACI Mix Design
� Step 9 - Adjustment for Moisture in the aggregate• The water content of the concrete will be
affected by the moisture content of the aggregate.
54
ACI Mix Design
� Step 9 - Adjustment for Moisture in the aggregate• The weight of aggregate from the stockpile is:
Weight(stockpile) = Weight(Oven dried) (1 + Moisture Content)
• The change in the weight water due to the moisture of the aggregate from the stockpile is:
∆Weight(water) = Weight(Oven dried) (Surface Moisture)
• Adjusted Weight(water) = Weight(water) – ∆Weight(water)
55
ACI Mix Design
� Step 9 - Adjustment for Moisture in the aggregate• Fine aggregate required from the stockpile:
= 1,196 lb (1+3%+1.3%)= 1,247 lb/yd3 (740 kg/m3)
• Coarse aggregate required from the stockpile:= 1,701 (1 + 1%) = 1,718 lb/yd3 (1,019 kg/m3)
• Required mixing water:= 280 lb – 1,196 lb x (4.3% - 1.3%) -
1,718 lb x (1% - 1%)= 244 lb/yd3 (145 kg/m3)
56
ACI Mix Design
� Estimated batch weight• Cement: 700 lb/yd3 (415 kg/m3)• Water: 244 lb/yd3 (145 kg/m3) • Coarse Agg: 1,718 lb/yd3 (1,019 kg/m3) • Fine Agg: 1,247 lb/yd3 (740 kg/m3)• Total: 3,909 lb/yd3 (2,319 kg/m3)
57
ACI Mix Design
� Step 10 - Trial Batch • Using the proportions developed in the
preceding steps to mix a trial batch of concrete.• The fresh concrete shall be tested for slump, unit
weight, yield, air content, and its tendencies to segregation, bleeding and finishing characteristics.
• Hardened samples shall be tested by compressive strength and other characteristics.
58
Volumetric Method
� Can be used to proportion high performance concrete mixture by incorporating admixtures
� Easily adopted from adequate past experiences and knowledge in the properties of raw materials used
Volumetric Method
� Past experiences and knowledge in:• relationship between strength and w/c ratio• grading and hardness of aggregates• proportion of total fine content in different
workability• suitably select admixture to minimize total
cementitious materials used• matrix performance for different proportion of
cementitious materials used
Volumetric Method
� The principal is the volume of compacted concrete equal to the sum of the absolute volume of all ingredients
� Require to know the density of all ingredients used
� Formula used:
Density = Mass/Volume
Volume (m3) = Mass (kg)/Density (kg/m3)
Volumetric Method
� Included air content (entrained and entrapped air), normally 0.8~1% in the mix design
� Aggregates are based on saturated - surface-dry (SSD) conditions
Volumetric Method
� In general, density (kg/m3) of local raw materials used in the mix design:
Cement (OPC) ~ 3,150
PFAGGBS
~ 2,400~ 2,900
Silica Fume (condensed) ~ 2,500
Coarse 20mm & 10mm in SSD ~ 2,600
Crushed rock fines in SSD condition
~ 2,600
Potable water 1,000
Admixtures depends
Volumetric Method
� General parameters (Examples) based on past experiences/trial results
� OPC 52.5N
� PFA not included
� Max. aggregate size is 20mm
� Dosage of normal water-reducer (lignin based) admixture in 0.8~0.9 L/100 kg cement)
Example:� Specified requirement: same as BRE method
mentioned above (i.e. Design 45D/20, 100mm slump)� Using the general parameters as the table listed
above and the following equation for 1m3 concrete,
(C/3150) + (Aggc/2600) + (Aggf/2600) + (W/1000) + (Am/1100) + Ac = 1 m3
where, C = cement content (kg)Aggc = total “20mm + 10mm” aggregates content (SSD) (kg)Aggf = crushed rock fine aggregate content (SSD) (kg)W = water content (kg)
Am = admixture content (kg), use density = 1100 kg/m3
Ac = air content (0.8~1%)
Volumetric Method
Volumetric Method
Step 1:Determination of cement content (C)
Water content is about 200 kg/m3
and W/C = 0.42, thusCement content C = 200 / 0.42
= 476 kg
Step 2:Determination of admixture content (Am)
Provide 0.85 L/100 kg cement of admixture, where S.G.= 1.10, thusAdmixture contentAm = (0.85 x 4.76) x 1.10
= 4.45 kg
Volumetric Method
Step 3:Determination of crushed rock fines content (Aggf)
The cohesiveness and workability required in the mix depends also on the total fine content (i.e. all cementitious materials + total fine aggregates content). In general, for 100mm slump, total fine content is about 0.40(~40% in volume). That is(C/3150) + (Aggf/2600) = 0.4(476/3150) + (Aggf/2600) = 0.4Aggf = 647 kg
Volumetric Method
Step 4:Determination of total coarse aggregates (20mm+10mm) content (Aggc)
(C/3150) + (Aggc/2600) + (Aggf/2600) + (W/1000) + (Am/1100) + Ac = 1 m3
For air content Ac = 0.9% = 0.009, thus, we have,
(476/3150) + (Aggc/2600) + (647/2600) + (200/1000) + (4.45/1100) + 0.009 = 1 m3
Aggc (20mm+10mm) = 1,006 kg
Volumetric Method
Step 5:Determination of each 20mm (Agg20) & 10mm (Agg10) contents
Generally, 10mm aggregates (Agg10) is about ~20% to total aggregates content (i.e. coarse + fine)Using 20%, we have,Agg10/(Aggc + Aggf) = 0.2Agg10/(1006 + 647) = 0.2Agg10 = 331
So, Agg20 = 1,006 – 331= 675 kg
Volumetric Method
Mix with OPC
Preliminary Mix Design Proportion
OPC = 476 kg/m3
20mm = 675 kg/m3
10mm = 331 kg/m3
CRF = 647 kg/m3
Water = 200 kg/m3
Admixture = 4.45 kg/m3
Wet density = 2,333 kg/m3
W/C = 0.42
Design Verification
� No matter using which concrete mix design method, trial mix is required to verify the design proportion.
� Design the mix proportions is a starting point.
� During trial mix stage, adjustment may be required to optimize the design mix proportion to suit the actual materials performance and specific applications.
� Further test to determine compatibility of materials and confirm the mix design.
� Field trial for final verification.
� Validate through production.
Theoretical Vs Laboratory Vs Field
Factors Affecting Mix Design
� Materials fluctuations� Insufficient batching & placing� Improper curing� Poor compaction� Testing� Site condition and malpractice
72
Difficulties & Constraints
� Concrete is not magic and still have its limitations although there is great improvement in concrete technology
� Concrete gain strength through cement hydration process and it takes time.
� Contradictory specification requirements �e.g. high compressive strength but low tensile splitting
strength�high PFA content but have to achieve high early
strength�…
73
Difficulties & Constraints
� Limited space in concrete batching plant for storage and handling of constituent materials.
� Stringent regulatory requirements and approval process for relevant permit and license.
� Sustainable materials supply e.g. aggregate supply.
74
Quality Management System
• Good quality concrete not only the responsibility of Concrete Producers.
• Concrete Producers have the ability to design and produce high standard concrete comply with specifications and requirements to suit the site applications.
• However, workmanship of concreting, compacting, curing cause significant impact to the performance of concrete.
75
Quality Management System
76
Good Quality
Concrete Mix
Concrete Producer
Testing Laboratory
Contractor
Consultant & Engineer
Architect
Quality Management System
• A stringent and high degree of quality control system among the Concrete Producers, Architects, Consultants, Engineers and Contractors shall be established
• The system ensure the high standard concrete to be specified, produced, placed, compacted and cured properly to achieve the desire performance and long term engineering benefits
77
Quality Management System
• Improper curing cause deterioration of strength development and durability of concrete
78
Quality Management System
• Impact of poor compaction• The presence of voids in concrete greatly reduces its
strength• Indicative figure show that 5% of voids can lower the
strength by as much as 30% even 2% voids can result in a drop of strength of more than 10%.
79
Final Words
• Concrete Producers in Hong Kong are capable for design and production of concrete mixes which fully comply with project requirements
• However, since the overall process is under very strict control, production rate is quite often compromised substantially and higher cost is thereby incurred.
• The concrete performance not only the concrete itself.
• A stringent and higher degree of quality control system among the Concrete Producers, Architects, Consultants, Engineers and Contractors is required
80
~ End ~
Thank You
81